Vol. 6, No. 3, 2003 Characterization of Corrosion Products Formed on Steels in the First Months of Atmospheric Exposure 403Materials Research, Vol. 6, No. 3, 403-408, 2003. © 2003
Characterization of Corrosion Products Formed on Steels in the First
Months of Atmospheric Exposure
Renato Altobelli Antunesa, Isolda Costaa, Dalva Lúcia Araújo de Fariab
aInstituto de Pesquisas Energéticas e Nucleares (IPEN),
Av. Prof. Lineu Prestes 2242, 05508-000, Butantã, São Paulo - SP, Brasil
bInst. de Química da Universidade de São Paulo (IQUSP),
05508-900 São Paulo - SP, Brasil
Received: September 25, 2002; Revised: April 13, 2003
The corrosion products of carbon steel and weathering steel exposed to three different types of
atmospheres, at times ranging from one to three months, have been identified. The steels were
exposed in an industrial site, an urban site (São Paulo City, Brazil), and a humid site. The effect of
the steel type on the corrosion products formed in the early stages of atmospheric corrosion has
been evaluated. The corrosion products formed at the various exposure locations were character-
ized by Raman microscopy, X-Ray diffraction (XRD) and their morphology was observed by
Scanning Electron Microscopy (SEM). Three regions of different colours (yellow, black and red)
have been identified over the steel coupons by Raman microscopy. Analysis carried out on each of
these areas led to the characterization of the correspondent oxide/hydroxide phases. The main
phases present were lepidocrocite (γ-FeOOH) and goethite (α-FeOOH). Small amounts of mag-
) were also eventually encountered.
Keywords: corrosion products, Raman microscopy, X-ray diffraction
ules (sandy crystals) or like fine plates (flowery structures).
The goethite looks like globular structures, called cotton
balls (semicrystalline goethite), interconnected by forma-
tions as nests or even like acicular structures (crystalline
goethite). The magnetite comes out as dark flat regions, with
However, despite the several works in this area there is
still little information about the steel oxide phases formed
in Brazilian tropical sites. The aim of this investigation was
to identify the components of the oxide layer formed on
coupons of carbon and weathering steels, exposed to at-
mospheric corrosion for periods from one to three months,
in three different atmospheres (a humid site located in a
tropical forest area, an industrial site and a densely popu-
lated urban site) in São Paulo, Brazil. The techniques used
for corrosion products characterization were X-ray diffrac-
tion and Raman microscopy.
Two types of steels were used in this study: a carbon
steel and a weathering steel. Their chemical composition is
The chemical characterization of the oxide layer formed
on metals and the understanding of its formation mecha-
nisms are important factors for the development and im-
provement of materials corrosion resistance.
Weathering steels contain alloying elements such as
copper, chromium and silicon that improve their corrosion
resistance comparatively to carbon steels1.
Many authors2-9 have studied the corrosion products
formed on carbon and weathering steels exposed to various
atmospheres by X-ray diffraction and Raman microscopy.
The main phases reported are lepidocrocite (γ-FeOOH),
goethite (α-FeOOH) and magnetite (Fe3O4). Lepidocrocite
is usually formed in the early stages of atmospheric corro-
sion3 but as the exposure time increases it is transformed
The morphology of the oxide layer formed on carbon
and weathering steels has been observed by several au-
thors10-14. The phases more frequently found (lepidocrocite,
goethite and magnetite) present typical structures. For in-
stance, the lepidocrocite appears like small crystalline glob-
404 Antunes et al. Materials Research
presented in Table 1. The chemical analysis was carried out
according to standard NGP 360006, using an equipment
ICP Optima 3000DV/ Leco Cs444.
Coupons of 150 × 100 mm were used for atmospheric
exposure. They were degreased with carbon tetrachloride
and blasted until a finishing Sa 2 1/2, according to
SIS SS 05590015.
Three atmospheres were used in the corrosion tests, spe-
cifically: Cubatão - SP, (industrial atmosphere), Alto da
Serra, also in Cubatão - SP (an humid site located in a tropi-
cal forest area), and at Paula Souza Street, in Sao Paulo city
(densely populated urban area).
The coupons exposure was carried out according to
ASTM G50-7616. At increasing times, one specimen of each
steel was taken from each atmospheric site and their corro-
sion products were characterized by X-ray diffraction and
Raman microscopy. In this paper only results correspond-
ing to one, two and three months of test are presented.
X-ray diffraction analysis was carried out with a Rigaku,
model DMAX-2000 equipment, using Cu-Kα radiation.
X-ray diffraction spectra were obtained directly on the speci-
men surface. For X-ray difraction analysis specimens of
10 × 20 mm were cut from the coupons whereas for Raman
microscopy and Scanning Electron Microscopy they were
15 × 15 mm in size. Raman spectroscopy was undertaken
using a Renishaw Raman microscope (System 3000), cou-
pled to an Olympus metalographic microscope and fitted
with a CCD detector (Wright, 600 × 400 pixels). The speci-
mens were excited with the 632.8 nm line from an air cooled
He-Ne laser (Spectra Physics, mod. 127). A 80× lens was
used to focus the laser (ca. 0.4 mW) on the samples and to
collect the scattered light.
SEM was carried out with a XL20 Phillips equipment.
The samples were covered with a gold film prior to the ob-
3. Results and Discussions
3.1 Raman Microscopy
All specimens analysed by Raman microscopy showed
regions of three different colors, yellow, red and black. Three
spectra were obtained for each of these regions, in three
different areas: at the center and closer to the borders. A
total of nine spectra were obtained for each specimen: three
of the yellow areas, three of the red and three of the black
areas. The results shown are characteristic of each region,
for each specimen.
The products identified in the oxide layer of carbon or
weathering steel exposed to the three sites (Alto da Serra,
Cubatão and Paula Souza) were lepidocrocite (γ-FeOOH),
goethite (α-FeOOH) and magnetite (Fe3O4). This was ob-
served for all the three exposure times reported in this pa-
per (one, two and three months). Since the corrosion prod-
ucts characterization by Raman microscopy was performed
in a small area (laser spot of ca. 4 µm2), a quantitative con-
tribution of each phase found is not possible even probing
different regions. However, it was possible to associate the
color of the oxide to a particular phase. It was found that
the red oxide showed Raman spectra typical of lepidocrocite
(γ-FeOOH), as reported in a previous work17, with the most
intense bands at 245 and 375 cm-1 18-22. Figure 1 shows a
representative lepidocrocite spectrum, for a specimen of car-
bon steel exposed at Alto da Serra site for three months.
The Raman spectra of yellow oxides indicated that they cor-
respond to a mixture of lepidocrocite and goethite (most
representative bands at 245, 299, 385, 479 and 550 cm-1 18-22).
In spite of some band overlapping (particularly the 245 cm-1
mode) the spectra allow an unequivocal differentiation be-
tween goethite and lepidocrocite. Figure 2 shows a spec-
trum typical of yellow regions, obtained from a weathering
steel specimen exposed to Paula Souza site for one month.
The black oxides showed Raman spectra with bands of
magnetite at 662 and 535 cm-1 together with lepidocrite and
goethite bands (Fig. 3). Magnetite is a black oxide17 and
therefore its detection on black areas is not surprising. The
spectrum shown in Fig. 3 was obtained from black areas on
carbon steel exposed for two months at Cubatão.
Similar spectra were obtained at black areas for all the
three exposure times (one, two and three months), both on
carbon or weathering steels, independently of the atmos-
pheric sites (Alto da Serra, Cubatão and Paula Souza).
3.2 X-Ray Diffraction
For oxide identification the JCPDS23 system was used,
after estimating the distance between the planes and the in-
tensity relative to each phase. A common feature in all X-
ray diffractograms obtained, either for carbon steel or weath-
ering steel, is the predominance of lepidocrocite, goethite
Table 1. Chemical composition of steels used.
Type of steel
Composition (weight %)
C S Al Cu Mn P Si Cr
C steel 0.037 0.009 0.,062
Vol. 6, No. 3, 2003 Characterization of Corrosion Products Formed on Steels in the First Months of Atmospheric Exposure 405
(α-FeOOH) and hydrated maghemite (γ-Fe2O3.H2O). Re-
flection lines corresponding to hematite (Fe2O3) have also
been observed in many specimens. Akaganeite (β-FeOOH)
was found on some specimens of weathering steel exposed
at Cubatão site.
In many specimens magnetite (Fe3O4) or maghemite
(γ-Fe2O3) were detected. The diffraction pattern for these
two oxides are very close and based only on X-ray diffrac-
tion results it is difficult to determine whether a mixture or
just one compound is present. Peaks relative to maghemite
were not detected by Raman microscopy, but magnetite was
found in many specimens. Therefore it is more likely that
the peaks (reflection lines) observed in the X-ray diffrac-
tion spectra are due to magnetite rather than to maghemite.
It cannot be ruled out, however, that maghemite also